HAL Id: hal-01290215
Submitted on 17 Mar 2016
HAL is a multi-disciplinary open access
archive for the deposit and dissemination of
sci-entific research documents, whether they are
pub-lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.
Quantitative assessment of the interfacial roughness in
multi-layered materials using image analysis:
Application to oxidation in ceramic-based materials
Sabine Le Roux, Frédéric Deschaux-Beaume, Thierry Cutard, Philippe Lours
To cite this version:
Sabine Le Roux, Frédéric Deschaux-Beaume, Thierry Cutard, Philippe Lours. Quantitative assessment
of the interfacial roughness in multi-layered materials using image analysis: Application to oxidation
in ceramic-based materials. Journal of the European Ceramic Society, Elsevier, 2015, 35 (3),
pp.1063-1079. �10.1016/j.jeurceramsoc.2014.09.027�. �hal-01290215�
assessment of the interfacial roughness in multi-layered
using image analysis: Application to oxidation
, T. Cutard1
1 Université de Toulouse, Mines Albi, INSA, ISAE, UPS, ICA (Institut Clément Ader); Campus Jarlard, F-81013 Albi cedex 09, France 2 Laboratoire de Mécanique et Génie Civil (LMGC), Université de Montpellier, CNRS, Montpellier, France
A method is developed to characterize interfacial roughness of layered materials. A series of contiguous images is acquired with a Scanning Electron Microscope on polished cross-sections. Using image analysis algorithms based on mathematical morphology operations, interface profiles are extracted and mathematically processed to calculate standard surface roughness parameters. In addition, morphological criteria describing the interface tortuosity are determined, such as the “normalized rumpling index” (based on the profile developed length) and the “barbule density” that quantifies the protrusions of the layer (using the skeletonization function). The validity and accuracy of the method is evaluated by comparison with measurements performed by the conventional surface metrology techniques. This method is used to study internal oxidation of two ceramic-based materials (Si3N4–TiN composite/thermal barrier coatings) upon thermal aging. In both cases, a link is established between the roughening of the oxide layer interface and a decrease in the mechanical strength of the multi-layered material.
Keywords: Interfacial roughness; SEM image analysis; Thermal aging; Oxidation; Thermal barrier coating systems
As a material is subject to a thermal aging or thermo-mechanical loading, an oxide layer generally grows at the surface, whose nature, thickness and morphology depend on the composition of the substrate material, the temperature and expo-sure time, and the applied or residual stresses. It is well known that the presence of a corrosion layer locally alters the intrin-sic properties of the material, often impacting its mechanical strength.1–6To prevent such premature damage of the material, it can be useful to deposit a protective coating on its surface (by CVD, PVD, plasma spraying, laser cladding or sputter-ing, sol–gel process, etc.). It was largely demonstrated that whatever the coating nature and the deposition process, the
∗Corresponding author. Tel.: +33 563493057; fax: +33 563493099.
E-mail address:firstname.lastname@example.org(S. Le Roux).
initial roughness of the substrate strongly influences the bond-ing mechanisms and the adhesion strength of the coatbond-ing,7–11 by favoring the mechanical anchoring on the substrate. On the other hand, both oxide and protective layers create an inter-nal interface with the base material, that undergoes chemical or morphological changes during the oxidation/coating process, or under the effect of thermal or thermo-mechanical loading. The interfacial “roughness” – which may vary depending on the oxi-dation/coating conditions – probably affects the layer adhesion to the substrate, and therefore the mechanical behavior of the material when submitted to a strong thermal gradient, a mechan-ical loading or wear. In the particular case of thermal barrier coating (TBC) systems or compositionally graded materials, several interfaces can be observed.12,13 Several authors12–15 have reported that a disrupted interface of the aluminide bond coat, which constitutes a site of high stress concentration, can promote failure mechanisms by large-scale spallation or delami-nation of the coating during cyclic exposure at high temperature. Therefore, it can be relevant to characterize the morphology of the weak interface beside other microstructural properties (such
as the phase transformations, the coating thickness, etc.), in order to better understand and predict the durability of such multi-layered materials (and especially the coating adherence) under thermal or mechanical stress.16–19
Quantifying surface roughness of an external layer is easy and straightforward, using conventional measuring devices such as mechanical probe instruments (contact stylus profiler, Atomic Force Microscope) or non-contact optical sensors (white-ligth or laser extended field confocal microscope, scanning inter-ferometer, optical scatterometer).20 Different resolutions and measurement ranges can be achieved depending on the mea-suring technique, and must be selected considering the nature of the material and the required accuracy.21,22Such devices are however inappropriate to characterize the morphology of sub-layers, since they do not allow access to the internal interfaces. In this case, a microstructural analysis is required, based on metal-lographic observations of cross-sections of the multi-material. The layer interface can be highlighted using an optical or scan-ning electron microscope (SEM), depending on the investigated scale of observation and the nature of the contrast between the different constituents of the layered material. However, these observations remain most often qualitative, even if some mathematical tools (like the fractal dimension D established by Mandelbrot23,24 or the correlation function of the Fourier spectrum25) can help to characterize the complex geometry of fracture surfaces,26–28 or to evaluate the adhesive strength of coatings.10 Tolpygo et al.14 employed a non-destructive technique, based on the photostimulated luminescence spec-troscopy, to monitor the damage and morphological changes of a layer interface during thermal aging or cycling. But even if the frequency shift observed on luminescence spectra provides interesting information, it remains insufficient alone to char-acterize and interpret unambiguously the layer damage. Using image analysis, the same authors29also quantified the top surface roughness and undulation of bond coats through quantitative parameters such as the RMS and the “tortuosity ratio” (corre-sponding to the lineal roughness). However, the detection of an internal interface is usually more complex, due to the presence of several layers or phase transformations in the micrographies. This paper proposes a methodology for quantitative morpho-metric analysis of interface(s) in layered materials, based on image analysis of SEM micrographs in cross-section. An algo-rithm is developed using mathematical morphology operations30 in order to extract the interface profile, which is mathemati-cally processed to separate roughness from waviness. Various morphological criteria and standard surface parameters are then calculated to evaluate the roughness and the corrugation of the profile. The validation of this method is provided by compar-ison with conventional measurements performed with a stylus profiler and a white light extended field confocal microscope. A first application, aiming to investigate the effect of oxidation on the mechanical behavior at high temperature of a non-oxide ceramic composite, is presented. The second application deals with the evolution of the oxide ratcheting and interface rum-pling of EB-PVD TBC systems as a function of thermal aging conditions. Data resulting from these investigations can be used beneficially to implement mechanistics models for achieving
a complete analysis of the local high temperature mechanical behavior of multi-layered materials. In such a case, this would require also to include microstructural features (size and crystal orientation of grains, voids and porosities, etc.) which are not deliberately considered here.
2. Experimental methodology
2.1. Sample preparation and SEM observation
In order to observe the oxide layer or the coating in cross section, the material is cut in the transverse direction and coated in a thick resin. Polished sections are prepared following classi-cal metallographic procedures. Then, the sample is observed in SEM using a back-scattered electron (BSE) detector. This allows to distinguish the various phases present in the material, which appear in different gray levels according to the atomic number of the chemical constituents. The parallelism between the sample surface and the horizontal border of the image is adjusted at a low magnification. Then, a higher magnification, which may vary depending on the layer thickness and morphology, is selected in order to highlight both the layer and the substrate/layer interface with sufficient accuracy (Fig. 1). A spatial resolution r≤ 1 m (i.e. near or better than lateral resolution commonly achieved with a conventional profiler) is required. This spatial resolution also reflects the height resolution (considering the amplitude of the profile along the z-axis), since the pixels of the image are square-shaped. A series of contiguous fields is recorded in order to represent the layer profile on an equivalent length of 4.8 mm (corresponding to the scanning length lt recommended by the
surface metrology standard).31 The total number N of images to acquire depends on the magnification factor, which must be selected in order to have a high enough spatial resolution. The size of the image (i.e. its number of pixels) can be an interest-ing adjustment parameter to reduce the magnification, but must however not be too large in order to optimize the processing time (as images with higher spatial resolution are longer to process).
2.2. Image analysis
Using the image analysis software Aphelion®, an algorithm is developed in order to extract the profile of the investigated surface (or interface) on each image-field of the series. In the example ofFig. 2, the detection of the top oxide layer profile consists in five steps. First, the contrast of the initial SEM image (Fig. 2a) is enhanced by applying a square function using look-up table (Fig. 2b). Then, the oxide layer is detected by gray level thresholding, based on the difference in phase contrast in the BSE image (Fig. 2c). The resulting binary image may contain noise (here some holes due to black porosities in the ceramic matrix) which must be “cleaned” using mathematical morphology operators, such as closing and hole filling operators (Fig. 2d). The next step aims to extract the surface or interface profile by applying an erosion of size 1 to image (d) (Fig. 2e), then a logical difference between images (d) and (e) (before and after erosion, respectively). This results in representing the surface profile as a continuous line of one pixel-thick (Fig. 2f).
Fig. 1. Procedure for SEM image acquisition: in this example, a series of 10 images is scanned along the layer on a total length (lt) of 4.8 mm (the covering area
between two adjacent fields is of about 10%).
Fig. 2. Image analysis procedure to extract the profile of the top oxide layer thermally grown on a ceramic composite (Si3N4–TiN): (a) initial SEM image with a
magnification of×1500, showing a phase contrast (BSE detector); (b) contrast enhancement by applying a square LUT; (c) gray-level thresholding; (d) cleaning of the binary image by morphological operations (closing and hole filling of porosities); (e) erosion of size 1, removing one pixel on the contour of the binary object; (f) detection of the profile of the top oxide layer by logical difference of binary images (d) and (e).
Finally, the list of points composing the profiles extracted from each image is saved in an ASCII file, as a table of two colums (abcissa x and height z(x), both expressed in pixels).
2.3. Mathematical processing of the proﬁles
The ASCII profile files extracted from the N images are processed using the mathematical software Matlab®. The first step consists in editing a single file gathering the data of all profiles, by ensuring the proper matching between the coordi-nates (abscissa x and height z) of the last point pfof the profile
extracted in the image j and those of the first point p1of the
pro-file extracted in the image (j + 1). For instance, each x(pi) value
of the profile (j + 1) is corrected by adding x:
Δx = x(pf)j− x(p1)j+1+ 1 (1)
The vertical offset along z-axis which may exist between two adjacent images must also be corrected, by adding z to each
z(pi) values of profile (j + 1) as follow:
Δz = z(pf)j− z(p1)j+1. (2)
At this stage, the total profile resulting from the assembly of the N profiles consists of a list of n connected points, whose
x and z coordinates are still expressed in pixels (Fig. 3a). It is therefore required to calibrate these values in micrometers, by multiplying each column (x,z) of the profile file by the spatial resolution r of the images. The resulting raw profile contains a range of spatial frequencies, from the form (low frequency com-ponents of large wavelength), the waviness (medium frequency components) to the actual roughness (high frequency irregular-ities). Forms errors, and especially the residual tilt of the profile with respect to the horizontal plane, can be removed by using a least-squares regression.32This method consists in choosing the
values of coefficients a and b to minimize the residue E (sum of square deviations), as expressed by the equations:
E = n i=0 ε2i = n i=0 (zi− (axi+ b))2, (3) with a = n n i=1 xi, zi− n i=1 xi n i=1 zi n n i=1 xi2− n i=1 xi 2 and b = n i=1 zi n − a n i=1 xi n , (4) where n is the total number of points in the profile, xi is the
position of point i along the x-axis, and ziis the height of point i along the z-axis.
The primary profile, which results from the subtraction of the least-squares line to the raw profile, contains both waviness and roughness components (Fig. 3b). In order to separate this two ranges of wavelengths, the primary profile is filtered with a low-pass filter, as implemented by the convolution function:
m(x) = z × s(x), (5)
Fig. 3. Mathematical processing of the profiles: (a) total raw profile resulting from the assembly of the profiles extracted from the N contiguous images; (b) calibrated primary profile, leveled by least-squares regression (the sampling length is lt= 4.8 mm); (c) roughness profile (short wave profile components),
obtained by subtracting the mean line to the primary profile (the mean line is superimposed to the roughness profile). Note that the evaluation length is reduced to le= 4 mm.
where m(x) is the output filtered profile, z(x) is the input primary profile, and s(x) is the impulsional response of the filter.
Eq.(5)is applied using a sliding weighted kernel function, which allows to reconstruct the so-called “mean line” m(x) of the profile (corresponding to the reference line used for surface assessment).33,34According to the ISO 11562 standard,35 the
Effect of the image magnification and resolution on the calculated value of the fractal parameter Ld/Lp.
Image magnification Image horizontal length (pixels) Spatial resolution (m/pixel) Profile developed length (pixel) Ld/Lp
×500 818 0.124 1194 1.460 ×750 1228 0.083 1808 1.472 ×1000 1635 0.062 2408 1.473 ×1250 2048 0.050 3025 1.477 Mean value 1.470 Standard deviation 0.007 Coef. of variation (%) 0.510
most widely used filter is the Gaussian filter, whose weighting function34is given by:
s(x) = 1 αλc exp −π( x αλc )2 (6) where α is a constant (α = 0.4697), and λcis the cut-off
The ordinate of the mean line at each point of abscissa x0thus
results from the calculation of the weighted average of the profile points located on either side, the ordinate of each point being weighted by a value s(δ), function of its distance δ (=x − x0) at
the considered point, as described by the equation:
z(x)s(x0− x)dx (7)
Finally, the roughness profile r(x), corresponding to short wave profile components (Fig. 3c), is obtained by subtracting the mean line m(x) to the primary profile z(x):
r(x) = z(x) − m(x) (8)
The influence of the cut-off length on the roughness parame-ters and the necessity to choose an appropriate value in order to avoid distorsions has been largely emphasized.20,32,33In the fol-lowing applications, a cut-off value of 0.8 mm was selected, as provided by International Standard ISO 11562.35As mentioned above, the sampling length (lt) of the profile is 4.8 mm, so as lt= 6λc. However, the evaluation length (le) should be reduced
to 4 mm (le= 5λc), in order to eliminate distorsion effects at the
beginning and the end of the filtered profile by removing the first half and the last half cut-off length.34 It is also important to note that the Gaussian filter used here is designed to have a transmission ratio of 50% at λc. This allows to calculate the
waviness profile by simply subtracting the roughness from the primary profile.34
2.4. Determination of surface parameters
In order to provide a numerical evaluation of the surface, quantitative parameters can be calculated either on the straight-ened primary profile, or on the roughness/waviness profiles (based on the mean line produced by the filtering). The complex-ity of the surface or interface can be simply evaluated by the ratio of the developed length (Ld) along the profile to the projected
length (Lp) on the x-axis (i.e. the length of the image-field). This
dimensionless criterion Ld/Lp, expressed “in excess” relative
to 100%, reflects in fact the “tortuosity” of the primary pro-file. However, it can be regarded as a “fractal dimension”, since its value may also depend on the image resolution. A sensitiv-ity analysis was performed on SEM images sizing (712× 484) pixels,2 acquired on the ceramic sample at various magnifica-tion factors ranging from×500 to ×1250 (and therefore various spatial resolutions). A similar profile length is extracted at the same position on each image, in order to determine the tortu-osity ratio Ld/Lp(Table 1). One can observe that Ld/Lpslightly
increases with the image resolution, but not really significantly for the investigated magnifications (coefficient of variation lower than 1%). Nevertheless, it should be recommended to consider this parameter only when comparing images with an equivalent spatial resolution.
2D roughness and waviness parameters used hereafter, whose complete definition can be found in ISO 4287,36are calculated on the filtered profiles. The asperity height of the roughness profile is quantified by amplitude parameters (such as Ra, Rz, Rt, Rq, etc. . .), all expressed in micrometers. As an example, the
mean roughness (Ra) measures the arithmetical average of the
absolute values of the profile height deviation from the mean line on the evaluation length. It can be expressed in the discrete case as: Ra= 1 n n i=1 |zi| (9)
where n is the number of data points on the evaluation length le,
and zithe distance between the height of point i and the mean
The root-mean-square roughness (RMS or Rq) calculates the
root mean square average of the profile height deviations from the mean line (i.e. the standard deviation of the height distribu-tion): Rq= 1 n n i=1 z2i (10)
The total height of the roughness (respectively waviness) pro-file, Rt(resp. Wt), measures the height between the highest peak
(Rp) and the deepest valley (Rv) within the evaluation length:
(11)Rt =max(Rpi) + |max(Rvi)|
The peak density (RPc) is a spacing parameter which consists
in counting the number of peaks over the evaluation length, and normalizing it on a length of 1 cm. A peak is counted each time
Standardized roughness parameters measured by mechanical profilometry on Si3N4-TiN samples oxidized at 1150◦C in air for various durations (mean values
calculated on 51 profiles).
Oxidation time Roughness parameters (m)
Ra Rq Rz Rmax Rt Rp Rv RSm RPc
1 h 1.37 1.77 10.7 13.0 13.7 7.35 3.35 26.1 32.7 10 h 2.00 2.61 13.5 15.7 16.0 10.2 5.80 34.0 28.8 50 h 2.30 2.91 15.4 18.0 18.7 7.20 7.30 35.0 30.1 100 h 2.83 3.56 18.3 21.2 22.0 13.3 8.30 83.0 24.5
the profile consecutively crosses the lower (C2) and upper (C1)
cutting depths, placed symmetrically on either side of the mean line (here considered at±1 m).
The mean spacing of irregularities (RSm) defines the mean
value of the width XS of the profile elements (consisting in a profile peak and the adjacent valley):
(12)RSm= m1 m
XSiwhere m is the number of profile
ele-ments within the evaluation length.
RSmgives the length of the period in the case of a periodic
or pseudo-periodic profile.
The skewness of the profile (RSk) is the quotient of the mean
cube value of the ordinate values z(x) and the cube of Rqwithin
the evaluation length:
RSk = 1 Rq3 1 n n i=1 z3i (13) RSkis an adimensional parameter which provides a
descrip-tion of the asymmetry of the profile. RSkis close to zero for a
Gaussian heigth distribution, whereas a positive value indicates a flat surface with peaks, and a negative value a bearing surface with valleys.
3. Validation of the method
To assess the reliability and performance of the roughness quantification using image analysis, comparative measurements were performed by conventional profilometric technics. For this purpose, three Si3N4–TiN ceramic samples thermally aged at
1150◦C in air for various exposure times (from 1 to 100 h) and providing different surface qualities of the superficial oxide layer, are characterized. 2D roughness parameters are deter-mined according to ISO 4287.36
3.1. Measurements by stylus proﬁlometry
Mechanical (or stylus) profilometry consists in traversing at a constant velocity across the surface to measure with a stylus, whose vertical displacement is converted into an electric signal using an inductive transducer, and electronically amplified. The diamond tip stylus is cone shaped, with a 5m radius and a 90◦ angle. The measuring range of the skidless pick-up is±100 m, and its vertical resolution (along z-axis) is 10 nm. A scanning length ltof 4.8 mm is selected, with a sampling interval of 1m.
Fifty-one profiles, distant from 50m each other, are scanned
over the sample surface. Each profile is straightened by least-squares regression, in order to correct the misalignment of the measured surface with the reference plane of the traverse unit. Then, the leveled profiles are filtered by using an appropriate cut-off length (λc= 0.8 mm here), and roughness parameters are
calculated (Table 2).
It must be emphasized that the stylus curvature radius, which acts as a mechanical low-pass filter, produces a smoothing of the real surface.37 This results in the loss of high spatial frequen-cies (narrow crevices and sharp peaks) on the profile (Fig. 4). Thus, using a 5m/90◦tip, the surface features having an angle greater than 45◦ to the horizontal and crevices which are nar-rower than 10m cannot be accurately recreated. Therefore, roughness parameters such as the total height Rtor the maximal
height Rmaxdetermined from mechanical probe measurements
are always underestimated.
3.2. Measurements by optical proﬁlometry
The same ceramic samples are measured using an extended field confocal microscope AltiSurf520 (from Altimet®), which is an optical profiler based on the principle of chromatic coding. A white-light source is focused on the sample surface where it is reflected, and a chromatic lens splits the reflected signal into its constituent wavelength. The exact height of the focused point is converted by a spectrometer. A chromatic (350m range) sensor, with an axial resolution of 10 nm and a lateral resolu-tion of 4m, is used. A rectangular area of 4.8 mm × 2.5 mm is scanned with a sampling interval of 1m, a scanning speed of 1 mm/s and a sampling frequency of 1000 Hz, providing a 3D topographical view of the sample surface (Fig. 5). Rough-ness parameters, calculated on 501 profiles extracted on the 3D surface, are reported inTable 3.
3.3. Measurements by image analysis
For each sample, the profile of the oxide layer is detected by image analysis on a series of 36 contiguous SEM images, by applying the processing routine detailed inFig. 2. The pro-files extracted from each image are saved in an ASCII file, as a list of points with a spatial resolution of 0.25m. Then, the profiles are mathematically processed following the procedure detailed inFig. 3. However, in order to compare these results with those obtained by mechanical profilometry, an algorithm was developed to reproduce the “smoothing” effect of the stylus. The moving of a ball with a radius curvature of 5 mm is simulated
Fig. 4. Limitations of contact measurements, due to the mechanical low-pass filtering exerted by the stylus tip geometry: (a) simulation of the effect of the tip radius on the surface profile; (b) smoothed profile by removing shorter frequencies corresponding to sharp peaks and narrow valleys.
Fig. 5. Topographies of Si3N4–TiN ceramic samples performed with an extended field confocal microscope (only a partial view of 2 mm× 2 mm is shown in order
to better highlight surface defects): unaged polished ceramic (a); top oxide layer formed after aging at 1150◦C in air for 1 h (b), 10 h (c) and 100 h (d).
over the rough surface, in order to filter the surface asperities that cannot be detected by the conical probe tip (Fig. 4a). Then, the resulting “smoothed” profile is leveled and filtered using a Gaussian numerical filter.
Roughness parameters are calculated on profiles processed or not with the smoothing algorithm, as reported inTable 4. It can be observed that the smoothing of the profile slightly changes the parameter values, especially for rougher surfaces and spacing parameters (RSm, RPc). Globally, the amplitude parameters are
lowered (except average parameters such as Raand Rq), while
the mean spacing of profile irregularities (RSm) is increased due
to the loss of fine details in the surface profile.
3.4. Reliability and precision of the method
InTable 5are reported the mean relative differences on rough-ness parameters between measurements performed by image analysis and by conventional techniques (stylus and optical pro-filometry). As can be noted, the results provided by the image analysis method are closer to those obtained by white light
Standardized roughness parameters measured by white light confocal microscopy on Si3N4–TiN samples oxidized at 1150◦C in air for various durations (mean
values calculated on 501 profiles).
Oxidation time Roughness parameters (m)
Ra Rq Rz Rmax Rt Rp Rv RSm RPc
1 h 1.50 1.99 12.2 17.2 19.2 8.80 3.07 30.4 22.2 10 h 2.45 3.15 18.4 28.2 32.9 12.3 5.79 31.0 26.2 50 h 2.98 3.63 20.3 24.7 27.4 11.7 8.28 30.0 27.9 100 h 4.03 5.24 29.1 37.0 35.8 15.5 11.6 37.2 24.8
Standardized roughness parameters measured by image analysis on SEM cross-sections of oxidized Si3N4–TiN samples at 1150◦C.
Oxidation time “Smoothing” algorithm Roughness parameters (m)
Ra Rq Rz Rmax Rt Rp Rv RSm RPc 1 h No 1.57 2.14 12.5 16.2 16.8 9.98 3.14 24.3 26.6 Yes 1.64 2.21 12.4 15.9 16.5 9.64 3.24 32.6 22.4 Relative difference (%) 4.5 3.1 −0.7 −2.0 −2.0 −3.4 3.2 33.9 −15.8 10 h No 2.61 3.42 19.5 25.8 26.8 14.8 5.61 30.4 29.4 Yes 2.68 3.47 18.8 25.7 24.6 13.9 5.82 38.0 22.4 Relative difference (%) 2.6 1.5 −3.9 −4.6 −4.1 −5.8 3.7 24.7 −23.8 50 h No 2.88 3.62 19.9 23.7 26.9 12.2 7.04 33.5 24.5 Yes 2.85 3.56 18.5 22.4 23.7 11.3 6.56 41.6 19.7 Relative difference (%) −1.0 −1.7 −7.2 −5.1 −11.9 −7.8 −6.9 23.9 −19.6 100 h No 3.71 4.54 24.2 29.1 36.9 12.6 12.4 44.6 19.9 Yes 3.98 4.74 25.0 26.1 26.5 12.0 11.0 53.0 16.7 Relative difference (%) 7.3 4.4 3.1 −10.2 −28.1 −4.8 −11.4 18.9 −16.0
extended field confocal microscopy (with a difference always less than 20% and 10% on average). The difference found with the stylus profiler is greater, image analysis giving higher values of about 30% on average (and up to 60% on Rt), despite the
smoothing of the profile simulating the conical tip of the sty-lus. This result can be explained by the higher spatial resolution reached on the SEM images (0.25m instead of 1.2 m for the stylus), as it is also the case for the optical sensor (4m). This offsets the lower resolution along z axis (25 times larger than the theoretical axial resolution of conventional methods). In addi-tion, the fineness of detail reproduction is much better, as profile irregularities corresponding to “backtracking” can be restored (Figs. 2f and 4b). On the other hand, it should be emphasized that some errors may be introduced during the metallographic preparation of the sample. Thus, cutting and polishing opera-tions can locally cause tearing of the outer surface, resulting in a slight modification of the surface. This is especially true when the material is brittle, as often the case with an oxide layer. How-ever, such artefacts of preparation have a null or minor influence on the reproduction quality of the internal (sub-layer) interfaces, which are the final subject of this study. Anyway, the particu-larly good agreement with optical measurements indicates that roughness parameters can be evaluated with satisfying orders of magnitude with our method. In addition, evolution of the
roughness of the ceramic composite surface as a function of oxidation time is clearly highlighted, as shown inFig. 6.
4. Application to a thermally aged ceramic composite: effect of the “roughening” of the internal oxidation interface on the mechanical strength
4.1. Material and experimental procedure
The material is a silicon nitride (Si3N4) based ceramic
con-taining 30% volumic of titanium nitride (TiN) particles, named Kersit 601, and elaborated by powder sintering. This low-density composite material is a good candidate to replace molybdenum superalloys – which are very expensive and very reactive with oxygen – in hot forging dies operating at temperatures above 1000◦C. Indeed, its good thermal properties (low thermal expan-sion coefficient, high thermal conductivity), associated with high mechanical and corrosion resistances, make it suited to with-stand sudden temperature changes in service.38
In order to study the oxidation behavior of the ceramic com-posite, static isothermal tests are performed at 1150◦C in air on small samples with a polished surface (Ra= 0.23m), for
various times (from 1 h to 200 h). Then, the thermally aged sam-ples are prepared as cross sections, and observed with SEM
Comparison of the roughness parameters measured by image analysis and by conventional methods. Oxidation time Reference (conventional
Relative difference (%) on calculated roughness parameters
Ra Rq Rz Rmax Rt Rp Rv RSm RPc
1 h Mechanical (stylus) 19.9 24.7 15.4 22.1 20.4 31.0 −3.4 24.8 −31.6 Optical (confocal micr.) 4.9 7.4 2.0 −5.7 −12.6 13.5 2.1 −20.0 19.8 50 h Mechanical (stylus) 33.8 33.0 39.0 56.4 60.6 36.7 0.3 11.6 −22.2 Optical (confocal micr.) 6.5 8.7 6.1 −8.6 −18.4 20.7 −3.0 −2.0 12.2 50 h Mechanical (stylus) 23.9 22.3 20.2 24.7 26.7 56.7 −10.1 18.8 −34.6 Optical (confocal micr.) −3.2 −0.2 −1.7 −4.2 −1.8 4.2 −14.9 12.0 −12.2 100 h Mechanical (stylus) 40.6 33.1 36.4 23.2 20.5 −9.8 31.9 −36.1 −31.8 Optical (confocal micr.) −8.0 −13.4 −16.7 −18.8 −7.4 −18.8 6.6 19.7 19.9
Fig. 6. Comparative evolution of roughness parameters measured by image anal-ysis and conventional methods (mechanical and optical profilometry) on the surface oxide layer of oxidized ceramic samples at 1150◦C, vs. oxidation time: (a) mean roughness Ra; (b) mean spacing of profile irregularities RSm.
using a BSE detector. The oxidation mechanisms and kinetics are fully described in.38As shown inFig. 7, two oxidation layers of different nature and composition are formed:
- a very compact and quasi-continuous top layer, consisting mainly of TiO2(appearing in light gray) with lesser amounts
of a SiO2glassy phase (in mid gray),
- a porous sub-surface layer partially oxidized, consisting of titanium oxide and silicon oxynitride (appearing in dark gray),
which overcomes the two-phase core material (with TiN grains in white and Si3N4matrix in mid gray).
In parallel to the oxidation tests, four-point bending tests are performed at 1150◦C on parallelepiped polished specimens, pre-oxidized at 1150◦C in air for various durations, in order to determine the failure strength of the material according to the oxidation duration. An electromechanical press Instron 5800 with a maximum load capacity of 30 kN, equipped with a tubu-lar resistance furnace, is used. After holding the specimens at 1150◦C for various times (from 30 min to 100 h), the bending tests are performed with a speed of 0.2 mm/s until failure. At the end of the test, the specimen is cooled to room temperature at a rate of 10◦C/min, in order to avoid thermal shock.
The maximum stress experienced by the specimen is given by: σmax= 3 2 P(L − l) bh2 (14)
where P is the applied load (in N), L and l are the distances between upper and lower supports (40 mm and 20 mm, respec-tively) in the bending test, and b and h are the width and the thickness of the specimen (4 mm and 3 mm, respectively).
Fig. 5clearly indicates that the surface roughness of ther-mally aged Si3N4–TiN samples increases due to oxide growth.
This “roughening” can be quantified by image analysis. The profile of the top oxide layer is extracted on each field of the series of contiguous cross-sectional SEM images, by applying the processing algorithm described above (Fig. 2). Another algo-rithm is developed to detect the interface between the partially oxidized area and the bulk ceramic, based on their difference in microstructure. It consists of four steps, as detailed inFig. 8: (a) dilatation to expand the white grains (TiN phase) in the
non-oxidized area (Fig. 8a);
(b) thresholding of the gray levels corresponding to the undam-aged area, composed of white TiN grains relatively large (Fig. 8b);
Fig. 8. Image analysis procedure applied on the image ofFig. 2b, to detect the interface between the partially oxidized zone and the undamaged ceramic: (a) dilatation of size 1 to expand the white grains (TiN phase) in the non-oxidized area; (b) thresholding of the light intensities in the image (a); (c) morphological closing to connect the closest binary TiN grains; (d) detection of the non-oxidized area by mathematical morphology operations (hole-filling, erosion-reconstruction to remove the binary noise, and smoothing of the contour of the detected area by series of closing-opening); (e) extraction of the interface profile by logical difference between the image (d) and its eroded of size 1; (f) interface profile superimposed on the initial SEM image.
(c) connection of the closest thresholded grains and remov-ing of the binary noise, usremov-ing mathematical morphology operations (Fig. 8c and d);
(d) detection of the profile of the upper interface of the undam-aged area by a logical difference between the previous binary image and its eroded of size 1 (Fig. 8e).
Primary (unfiltered) profiles resulting from the image processing of the samples for various oxidation times are reported onFig. 9a and b, respectively for the upper oxide layer and the interface between the partially oxidized zone and the bulk ceramic.
4.2. Results and discussion
The thickness of the top oxide layer and of the partially oxi-dized area increases by increasing the oxidation time (Fig. 10).
Fig. 9a shows that the initially smooth surface develops rough-ness defects whose amplitude increases during oxidation, as
better reflected by the increasing trend versus oxidation time of the average surface roughness Ra (Fig. 11a). A gradual
roughening is also observed at the interface between the par-tially oxidized area and the undamaged substrate, and especially beyond 10 h of oxidation (Figs. 9b and 11a).
Due to the brittle nature of the ceramic material, the results of the bending tests are represented by the failure probability (Weibull distribution) as a function of the maximum stress suf-fered by pre-oxidized specimens for 0.5 h, 50 and 100 h (Fig. 12). As could be expected, the rupture probability is much higher when the oxidation time is longer and the tensile strength is reduced by about 100 MPa when the oxidation time is increased to 100 h. The decrease of the mean failure stress is then corre-lated to the increase of Raat the interface between the partially
oxidized area and the bulk ceramic during oxidation (Fig. 11a), that causes an increase of stress concentrations at the surface of the bulk material. The increased amplitude of waviness defects, maximum after 100 h (Fig. 11b), can also contribute to amplify this stress concentration effect, even if those higher wavelength
Fig. 9. Evolution the profile of the superficial oxide layer (a) and of the inter-face between the partially oxidized area and the bulk ceramic (b), for various oxidation times at 1150◦C (the profiles are vertically offset).
defects may produce a lesser “notch effect”.39It is well known that for brittle materials, the failure strength is directly corre-lated to surface or volume flaws distribution in the material. In the case of high strength Si3N4–TiN ceramic composites,
sur-face flaws become more critical than volume flaws when sursur-face roughness increases. As observed inFig. 7, the partially oxidized sub-layer is very porous, lowering its strength as compared to that of the bulk material. This is confirmed by the occurrence of oxide spallation generally observed along the interface between the bulk ceramic and the partially oxidized layer on post-mortem
Fig. 10. Oxidation kinetics of the Si3N4–TiN ceramic under thermal aging tests
in air at 1150◦C.
Fig. 11. Variation with the oxidation time of the profile irregularity of the top oxide layer and at the interface between the partially oxidized area and the bulk ceramic: (a) mean roughness Ra; (b) waviness depth Wt.
bending specimens. Then, we can suppose that the surface flaws responsible for the decrease of the failure strength of oxidized materials are located at the bulk material/partially oxidized zone interface. In addition,Fig. 12indicates that dispersion of failure
Fig. 12. Results of the room temperature 4-points bending tests performed on Si3N4–TiN specimens pre-oxidized at 1150◦C during 0.5 h, 50 and 100 h:
graphic representation of the probability of failure as a function of the rupture stress.
Fig. 13. Laminate structure and composition of the thermal barrier coatings elaborated by EB-PVD process.
stresses increases after 50 oxidation hours, and then decreases after 100 h. This can be related to the density of large surface flaws that systematically provokes fracture under low stress for long term exposure. As can be observed on the surface profiles of Fig. 9a, such surface defects are more numerous after 100 oxidation hours, increasing the risk of failure and thus reducing the fracture stress dispersion. On the contrary, there are few deep valleys after 50 hours exposure, which lowers the probability for initiating cracks on surface defects and explains the experimental values significantly scattered on the Weibull distribution.
5. Application to the oxidation of thermal barrier coating systems: relationship between the ratcheting of the thermally grown oxide and the interfacial adhesion
5.1. Material and experimental procedure
The investigated material is a thermal barrier coating (TBC) system deposited by EB-PVD (Electron-Beam Physical Vapour Deposition) on a nickel based superalloy substrate. The EB-PVD coating consists of three superposed layers (Fig. 13):
- a ceramic top coat of∼7% yttria-stabilized zirconia, acting as a thermal barrier,
- a slowly growing, adherent␣-Al2O3thermally grown oxide
(TGO), acting as a diffusion barrier,
- an alumina-forming (Ni,Pt)Al bond coat, which accomodates the differences in thermal expansion between the superalloy and the thermal barrier, thus enhancing the adherence of the top-coat.
Such TBC systems are used in the manufacture of aircraft engine blades, and especially in jet engine turbines to protect single crystal blades from both the corrosive attack of combus-tion hot gases and the extremely high temperature continuously increased to enhance engine efficiency. In service, this com-plex multi-layered structure is exposed to severe conditions, and the resulting thermo-mechanical loading is responsible for the degradation of the interfacial adhesion of the layers which may lead to a premature damage of the component.
We aim to investigate the thermal aging of the TBC sys-tem under static isothermal conditions, for 100 h at oxidation temperatures ranging from 1050 to 1150◦C. We focus on the alu-mina TGO layer, initially formed by the oxidation of aluminum drawn from the reservoir bond coat in contact with the oxygen of air. Indeed, the time and temperature dependent thickening of this layer during thermal aging or cycling develops signif-icant growth stress as well as rumpling and associated strain, possibly leading or at least contributing to the spallation of the thermal barrier coating. To assess the effect of the temperature on both the thickness and the wrinkling of the TGO layer, the ther-mally aged samples are prepared as cross-sections and observed in SEM (Fig. 14). The interfacial roughness of the TGO layer is quantified using Aphelion®on a series of 30 images-fields sizing (2048× 1887) pixels2 and aquired over a total length of 4.8 mm with a magnification of 750×. The image analy-sis algorithm, detailed inFig. 15, is composed of several steps including:
(a) a median filtering of the initial SEM image (Fig. 15a); (b) the thresholding of the dark gray levels corresponding to
the TGO layer. As can be observed inFig. 15b, some dark precipitates in the superalloy and big porosities in the upper ceramic are also detected;
(c) an hysteresis thresholding selecting only the precipitates and porosities (Fig. 15c);the removing of the binary noise by a logical difference between the images of Fig. 15b andFig. 15c. One can note that even if some unwanted details still remains inFig. 15d, it is disconnected from the layer of interest. The complete removal of residual noise is achieved by erosion-reconstruction with a structuring ele-ment of appropriate size, which allows the detection of the single layer (Fig. 15e);
(d) the extraction of both upper and lower profiles of the TGO layer by logical difference between the binary image of the layer and its eroded of size 1 (Fig. 15f). The upper (Pu) and
lower (Pl) profiles correspond to the interface between the
TGO layer and the ceramic layer, and between the TGO layer and the sub-layer covering the superalloy substrate, respectively.
The equivalent thickness (te) of the TGO layer can be
calcu-lated by dividing the area A of the layer (number of binarized pixels in the image ofFig. 15e) and the developed length Lm(in
pixels) of the median profile of the layer, as expressed by: (15)te= (A/Lm)r
Note that the result is calibrated, knowing the spatial resolu-tion of the image (r = 0.083m/pixel here).
As detailed inFig. 16, the median axis (line of 1 pixel width) is achieved by skeletonization of the TGO layer, followed by a pruning to convergence to remove the residual barbules of the skeleton.30Taking into account the median length Lm (instead
of the projected length Ld) in Eq. (15) provides a more accurate
estimation of the mean thickness of the TGO layer, since the median axis better reflects the “ratcheting effect”of the layer. In
Fig. 14. SEM observations showing the increased thickness and roughening of the TGO layer due to thermal aging: reference unaged sample (a) and thermally aged samples at 1050◦C (b), 1100◦C (c), and 1150◦C (d).
addition, the linear density of barbules (db) along the profile is
db= Nb/Ld (16)
where Nbis the number of barbules of significant size (>1m
In parallel, interfacial Vickers indentation are implemented, in order to determine the critical load required to initiate crack between the ceramic and the TGO layer and consequently to characterize the adhesion of the TBC system on the substrate material. The critical load is approached by first establishing both the “hardness master curve” and the “crack curve”, plotting respectively the indent size and crack size versus the applied force. It is then determined graphically by seeking the intercept, for each aging condition, between the two curves.40 In turn, the apparent toughness of the interface is calculated using the following expression: Kca = 0.015 Pc ac3/2 E H i 1/2 and E H 1/2 i = E H 1/2 S 1+ HS HTBC 1/2 i + E H 1/2 TBC 1+ HTBC HS 1/2 i , (17)
where subscript S, i and TBC stands respectively for the sub-strate, the interface and the TBC, Pcis the critical load (in N), ac
is the crack length (in m) at the critical load, E is the Young mod-ulus (200 GPa for the substrate, and 66 GPa for the TBC coating),
H is the hardness (550 HV, i.e. 5.39 GPa for the substrate, and
401 HV, i.e. 3.93 GPa for the TBC coating).
5.2. Results and discussion
As shown in Fig. 13b–d, the TGO layer grows and sig-nificantly changes its morphology upon isothermal oxidation. However, its upper (Pu) and lower (Pl) interfaces do not exhibit
the same evolution, Pubecoming progressively more corrugated
than Plas oxidation temperature is increased. To quantify this
morphological evolution, a normalized rumpling index (NRI) is defined as the ratio of the fractal parameter Ld/Lp(as detailed in
Section2.4) measured after thermal aging and initially before any temperature exposure:
NRI= (Ld/Lp)aged (Ld/Lp)unaged
Fig. 17 reveals that an increase in the oxidation tempera-ture from 1050 to 1150◦C results in a roughly linear increase of the NRI value, in particular at the interface between the TGO layer and the ceramic top coat. The roughening of the interface is also highlighted by the root-mean-square roughness
Rq(Fig. 18a), whose evolution indicates that the amplitude of
defects is strongly increased under the effect of the aging tem-perature, and especially above 1150◦C. A detailed statistical analysis further reveals that the distribution of defects changes along the TBC–TGO interface, as shown by the evolution of the skewness RSk(which expresses the asymmetry of the profile
relative to the mean line) versus the temperature (Fig. 18b). RSk
changes from initially near zero for the unaged sample to a neg-ative value for thermally aged samples. It can thus be inferred that the morphology of the TGO layer evolves by formation of deeper “valleys” (inward defects) upon thermal aging.
All these observations globally reflects an enhancement of the tortuosity of the interface between the TBC and the TGO
Fig. 15. Image analysis procedure to extract the upper and lower profiles of the TGO layer: (a) median filtering of the SEM image; (b) thresholding of the TGO layer; (c) thresholding of the precipitates “connected” to the TGO layer; (d) logical difference between images (b) and (c); (e) erosion-reconstruction of the image (d) to filter the binary noise; (f) detection of the profiles by logical difference between the image (e) and its eroded of size 1.
Fig. 16. Detection of the median axis of the TGO layer: (a) skeletonization of the layer; (b) pruning of the skeleton to remove residual barbules; (c) superim-position of the median profile on the TGO layer.
Fig. 17. Evolution of the normalized rumpling index (NRI), measured on lower (Pl) and upper (Pu) profiles of the TGO layer, as a function of the temperature
Fig. 18. Evolution versus aging temperature of roughness parameters at the interface between the TGO layer and the ceramic top coat: (a) root-mean-square
Rq, which indicates that the defect amplitude increases by increasing the
temper-ature; (b) skewness RSk, which expresses the asymmetry of the profile relative
to the mean line.
following cyclic exposure at high temperature. This structural change, so-called “rumpling”, results from the deformation of the underlying substrate subsequently to the accumulation of oxidation cycles and the associated thermal stress. The deformation may provoke the corrugation of the TGO at the TBC/substrate interface and the propensity of the system to develop rumpling is related to the capability of the deposit, according to its mechanical properties, to avoid or not the establishment of plastic strain under the stress state due to ther-mal cycling and TGO growth stress. Note that NRI is above 1 at the Pu interface, but lower than or close to 1 at the Pl
interface (Fig. 17). Consequently, rumpling of thermally aged samples appear to preferentially affect the TBC–TGO inter-face, which would be more prone to break. This is consistent with observations made by Tolpygo et al.29on similar EB-PVD TBC systems investigated under cyclic oxidation at 1150◦C. Rumpling is a consequence of the thermal expansion mis-match between the TGO layer (with a coefficient of thermal expansion α of 8–9×10−6 ◦C−1) and the upper and lower lay-ers (TBC coating with α = 11–13×10−6 ◦C−1 and bond coat with α = 13–16×10−6 ◦C−1), leading to alternating compres-sive/tensile stresses at the interfaces between the different layers. In addition, Fig. 19 indicates that the thickness of the TGO
Fig. 19. Evolution of the thickness and barbule density of the TGO layer as a function of the temperature of isothermal aging tests.
Apparent toughness Kcameasured at the interface between the TBC coating
and the substrate by interfacial indentation tests on samples oxidized at various temperatures.
Oxidation conditions Critical load Pc (N) Crack length ac (m) Apparent toughness Kac (MPa m0.5) Unaged 11.3 50.4 3.31 1050◦C–100 h 2.09 14.7 2.98 1100◦C–100 h 0.85 8.5 2.57 1150◦C–100 h 0.34 4.9 2.35
layer and the “barbule density” also increase as a function of the aging temperature. As illustrated in Fig. 16a, these bar-bules appear preferentially above the layer median axis. The increasing number of barbules with the oxidation temperature thus reflects the formation of local “protrusions”, due to a het-erogeneous growth of the TGO layer. This is probably related to the EB-PVD process, which favors a columnar grain growth in the ceramic surface layer and the formation of inter-columnar porosities.
In parallel, the apparent interfacial toughness Kac, measured
by interfacial indentation tests, drastically decreases upon ther-mal aging, lowering the adhesion of the TBC system over the substrate (Table 6). This suggests the existence of a relationship between the mechanical strength of the TBC system and the roughness of its interface with the substrate. It must however be emphasized that rumpling is not the unique cause responsi-ble for the failure of the TBC system. In fact, the thickness and chemical composition of the TGO layer, which vary depending on the aging temperature, may also influence the physical and mechanical properties of the coating, and therefore its adhesion to the substrate.14,29,41
The interfacial roughness of oxide layers or of thermal bar-rier coatings is investigated by image analysis on cross-sectional images. The procedure consists in acquiring a number of con-tiguous images-fields on a prescribed length, with an appropriate
magnification and resolution selected according to the required observation scale. Image analysis algorithms are developed to extract the profile(s) of the surface or internal layer based on the difference of microstructure. The profiles extracted from each image are saved in an ASCII file, assembled, and mathematically processed in order to be calibrated, leveled and filtered. Quanti-tative parameters are proposed to describe the roughness of the interface profile, like the fractal dimension Ld/Lprelative to the
normalized developed length, or conventional roughness param-eters (such as Ra, Rz, Rq, . . .) calculated according to the surface
metrology standards. The method is validated by comparative measurements by stylus profilometry and extended field con-focal microscopy, performed on the superficial oxidation layer thermally grown on a composite ceramic sample. The accuracy obtained is satisfactory and the representativeness of results is relevant. Finally, two application cases are exposed to show the potential information provided by this original method. The first one concerns the investigation of the effects of oxidation of a ceramic composite Si3N4–TiN thermally aged in air at 1150◦C
on its mechanical properties. It is shown that the strength of pre-oxidized specimens in bending tests is correlated to the inter-facial roughness of the partially oxidized layer. The second case study deals with the thermal aging of thermal barrier coating sys-tems elaborated by EB-PVD process. A relation is highlighted between the ratcheting of the bond coat interface (measured by roughness parameters) and the adhesion of the TBC sys-tem on the substrate (measured here by interfacial indentation tests).
Although it is destructive, the characterization technique developed is applicable to any kind of (multi-)layered materi-als, provided that the layer(s) of interest is (are) distinguishable either by optical or scanning electron microscopy. It provides a quantitative analysis of the interfacial roughness and/or wavi-ness of corrosion layers or surface coatings, difficult to reach by other conventional techniques, with good reproducibility and precision. In addition, it allows to estimate other relevant infor-mation such as the thickness of the (sub-)layer(s). Combined with mechanical characterization (such as interfacial indentation tests, flexure tests, laser shock waves, . . .), those morphological criteria can help to understand the mechanisms that govern adhe-sion of coatings deposited by any surface treatment process (such as CVD, PVD, plasma spraying, laser cladding, sol-gel process, etc.). However, note that the approach proposed in the paper does not include full consideration of microstructural details, in particular the density and evolution of interfacial defects and the substrate crystal characteristics (grain size, texture, etc.). Indeed, in order to accurately model the mechanical behavior of multi-materials with a gradient of composition, it would be of course necessary to take into account possible associated long range length scale effects.
The authors gratefully acknowledge Yinghui Liu and Serge Tovar for sample preparation and SEM observations, and Dr. Vanessa Vidal for fruitful discussions.
1.Cook RH, Skelton RP. Environment-dependence of the mechanical proper-ties of metals at high temperature. Int Mater Rev 1974;19(1):199–222.
2.Molins R, Hochstetter G, Chassaigne JC, Andrieu E. Oxidation effects on the fatigue crack growth behaviour of alloy 718 at high temperature. Acta
3.Chen TH, Weng KL, Yang JR. The effect of high-temperature exposure on the microstructural stability and toughness property in a 2205 duplex stainless steel. Mater Sci Eng A 2002;338(1):259–70.
4.Pather R, Mitten WA, Holdway P, Ubhi HS, Wisbey A, Brooks JW. The effect of high temperature exposure on the tensile properties of␥ TiAl alloys.
5.Deschaux-Beaume F, Cutard T, Fréty N, Levaillant C. Oxidation of Si3N4–TiN composites in air. Adv Sci Technol 1999;13:A389–96.
6.Dour G, Lamesle P, Salem M, Le Roux S, Rézaï-Aria F. Oxidation and corro-sion effects on thermal fatigue behaviour of hot work tool steel X38CrMoV5 (AISI H11). Mater Sci Forum 2008;595:789–96.
7.Sobolev VV, Guilemany JM, Nutting J, Miquel JR. Development of substrate-coating adhesion in thermal spraying. Int Mater Rev 1997;42(3): 117–36.
8.Staia MH, Ramos E, Carrasquero A, Roman A, Lesage J, Chicot D, et al. Effect of substrate roughness induced by grit blasting upon adhesion of WX-17% Co thermal sprayed coatings. Thin Solid Films 2000;377–378:657–64.
9.Wang YY, Li CJ, Ohmori A. Influence of substrate roughness on the bonding mechanisms of high velocity oxy-fuel sprayed coatings. Thin Solid Films 2005;485(1):141–7.
10.Amada S, Yamada H. Introduction of fractal dimension to adhesive strength evaluation of plasma-sprayed coatings. Surf Coat Technol 1996;78(1):50–5.
11.Habig KH. Wear behaviour of surface coatings on steels. Tribol Int 1989;22(2):65–73.
12.Evans AG, Mumm DR, Hutchinson JW, Meier GH, Pettit FS. Mecha-nisms controlling the durability of thermal barrier coatings. Prog Mater
13.Schulz U, Leyens C, Fritscher K, Peters M, Saruhan-Brings B, Lavigne O, et al. Some recent trends in research and technology of advanced thermal barrier coatings. Aerosp Sci Technol 2003;7(1):73–80.
14.Tolpygo VK, Clarke DR, Murphy KS. Evaluation of interface degradation during cyclic oxidation of EB-PVD thermal barrier coatings and correlation with TGO luminescence. Surf Coat Technol 2004;188:62–70.
15.Zhang D, Gong S, Xu H, Wu Z. Effect of bond coat surface roughness on the thermal cyclic behavior of thermal barrier coatings. Surf Coat Technol 2006;201(3):649–53.
16.Freborg AM, Ferguson BL, Brindley WJ, Petrus GJ. Modeling oxi-dation induced stresses in thermal barrier coatings. Mater Sci Eng A 1998;245(2):182–90.
17.Pindera MJ, Aboudi J, Arnold SM. The effect of interface roughness and oxide film thickness on the inelastic response of thermal barrier coatings to thermal cycling. Mater Sci Eng A 2000;284(1):158–75.
18.Ahrens M, Vaßen R, Stöver D. Stress distributions in plasma-sprayed ther-mal barrier coatings as a function of interface roughness and oxide scale thickness. Surf Coat Technol 2002;161(1):26–35.
19.Balint DS, Hutchinson JW. An analytical model of rumpling in thermal barrier coatings. J Mech Phys Solids 2005;53(4):949–73.
20.Whitehouse DJ. Handbook of surface and nanometrology. 2nd ed. Boca Raton: CRC Press; 2011.
21.Whitehouse DJ. Comparison between stylus and optical methods for mea-suring surfaces. CIRP Ann Manuf Technol 1988;37(2):649–53.
22.Poon CY, Bhushan B. Comparison of surface roughness measure-ments by stylus profiler, AFM and non-contact optical profiler. Wear 1995;190(1):76–88.
23.Mandelbrot BB. The fractal geometry of nature. Revised and enlarged ed. New York: WH Freeman & Co.; 1983.
24.Voss RF. Characterization and measurement of random fractals. Phys Scr 1986;T13:27–32.
25.Berry M, Hannay J. Topography of random surfaces. Nature 1978;273:573.
26.Mandelbrot BB, Passoja DE, Paullay AJ. Fractal character of fracture sur-faces of metals. Nature 1984;308:721–2.
27.Mecholsky JJ, Passoja DE, Feinberg-Ringer KS. Quantitative analysis of brittle fracture surfaces using fractal geometry. J Am Ceram Soc 1989;72(1):60–5.
28.Trefilov VI, Kartuzov VV, Minakov NV. Fractal dimension of fracture sur-faces. Met Sci Heat Treat 2001;43(3–4):95–8.
29.Tolpygo VK, Clarke DR, Murphy KS. On the rumpling mechanism in nickel-aluminide coatings: Part II: characterization of surface undulations and bond coat swelling. Acta Mater 2004;52(17):5129–41.
30.Serra J. Image analysis and mathematical morphology, Vol. 2. London: Academic Press; 1982.
31.International Standard ISO 4288. Geometrical Product Speciﬁcations (GPS)
– surface texture: proﬁle method – rules and procedures for the assessment of surface texture. Geneva: International Organization for Standardization;
32.Mummery L. Surface texture analysis—the handbook. 2nd ed. Muhlhausen (Germany): Hommelwerke GmbH; 1992.
33.Gurau L, Mansfield-Williams H, Irle M. Filtering the roughness of a sanded wood surface. Holz als Roh-und Werkstoff 2006;64(5):363–71.
34.Raja J, Muralikrishnan B, Fu S. Recent advances in separation of roughness, waviness and form. Precis Eng 2002;26(2):222–35.
35.International Standard ISO 11562. Geometrical Product Speciﬁcations
(GPS) – surface texture: proﬁle method – metrological characteristics of phase correct ﬁlters. Geneva: International Organization for
36.International Standard ISO 4287. Geometrical Product Speciﬁcations (GPS)
– surface texture: proﬁle method – terms, deﬁnitions and surface texture parameters. Geneva: International Organization for Standardization; 1997.
37.O’Donnell KA. Effects of finite stylus width in surface contact profilometry.
Appl Opt 1993;32(25):4922–8.
38.Deschaux-Beaume F, Fréty N, Cutard T, Colin C. Oxidation modeling of a Si3N4–TiN ceramic: microstructure and kinetic laws. Ceram Int
39.Wang F, Zheng XL, Lu MX. Notch strength of ceramics and statistical analysis. Eng Fract Mech 1995;52(5):917–21.
40.Sniezewski J, Vidal V, Lours P, Le Maoult Y. Thermal barrier coatings adher-ence and spallation: interfacial indentation resistance and cyclic oxidation behaviour under thermal gradient. Surf Coat Technol 2009;204(6):807–11.
41.Sniezewski J, Le Maoult Y, Lours P. Oxidation and spallation of FeCrAl alloys and thermal barrier coatings: in situ investigation under controlled temperature gradient. Mater High Temp 2010;27(2):101–8.